LMucko/crystallography-open-database huggingface dataset:
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide Locality: synthetic
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008052
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
 Locality: synthetic
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_formula_structural     Cd(NH3)2Cl2
_chemical_formula_sum            'Cd Cl2 N2'
_space_group_IT_number           35
_symmetry_space_group_name_Hall  'C 2 -2'
_symmetry_space_group_name_H-M   'C m m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.196
_cell_length_b                   8.307
_cell_length_c                   3.968
_cell_volume                     270.158
_exptl_crystal_density_diffrn    2.598
_cod_original_formula_sum        'Cd N2 Cl2'
_cod_database_code               9008052
_database_code_amcsd 0010556
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008053
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_structural     Cd(NH3)2Cl2
_chemical_formula_sum            'Cd Cl2 N2'
_space_group_IT_number           38
_symmetry_space_group_name_Hall  'A 2 -2'
_symmetry_space_group_name_H-M   'A m m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.968
_cell_length_b                   8.307
_cell_length_c                   8.196
_cell_volume                     270.158
_database_code_amcsd             0010557
_exptl_crystal_density_diffrn    2.598
_cod_original_formula_sum        'Cd N2 Cl2'
_cod_database_code               9008053
_amcsd_formula_title             Cd(NH3)2Cl2
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide Locality: synthetic
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008054
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
 Locality: synthetic
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_formula_structural     Cd(NH3)2Cl2
_chemical_formula_sum            'Cd Cl2 N2'
_space_group_IT_number           21
_symmetry_space_group_name_Hall  'C 2 2'
_symmetry_space_group_name_H-M   'C 2 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.196
_cell_length_b                   8.307
_cell_length_c                   3.968
_cell_volume                     270.158
_exptl_crystal_density_diffrn    2.598
_cod_original_formula_sum        'Cd N2 Cl2'
_cod_database_code               9008054
_database_code_amcsd 0010558
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide Locality: synthetic
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008055
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
 Locality: synthetic
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_formula_structural     Cd(NH3)2Cl2
_chemical_formula_sum            'Cd Cl2 N2'
_space_group_IT_number           65
_symmetry_space_group_name_Hall  '-C 2 2'
_symmetry_space_group_name_H-M   'C m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.196
_cell_length_b                   8.307
_cell_length_c                   3.968
_cell_volume                     270.158
_exptl_crystal_density_diffrn    2.598
_cod_original_formula_sum        'Cd N2 Cl2'
_cod_database_code               9008055
_database_code_amcsd 0010559
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide Locality: synthetic
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008056
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
 Locality: synthetic
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_formula_structural     Cd(NH3)2Br2
_chemical_formula_sum            'Br2 Cd N2'
_space_group_IT_number           35
_symmetry_space_group_name_Hall  'C 2 -2'
_symmetry_space_group_name_H-M   'C m m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.55
_cell_length_b                   8.55
_cell_length_c                   4.13
_cell_volume                     301.913
_exptl_crystal_density_diffrn    3.303
_cod_original_formula_sum        'Cd N2 Br2'
_cod_database_code               9008056
_database_code_amcsd 0010560
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008057
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_structural     Cd(NH3)2Br2
_chemical_formula_sum            'Br2 Cd N2'
_space_group_IT_number           38
_symmetry_space_group_name_Hall  'A 2 -2'
_symmetry_space_group_name_H-M   'A m m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.13
_cell_length_b                   8.55
_cell_length_c                   8.55
_cell_volume                     301.913
_database_code_amcsd             0010561
_exptl_crystal_density_diffrn    3.303
_cod_original_formula_sum        'Cd N2 Br2'
_cod_database_code               9008057
_amcsd_formula_title             Cd(NH3)2Br2
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide Locality: synthetic
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008058
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
 Locality: synthetic
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_formula_structural     Cd(NH3)2Br2
_chemical_formula_sum            'Br2 Cd N2'
_space_group_IT_number           65
_symmetry_space_group_name_Hall  '-C 2 2'
_symmetry_space_group_name_H-M   'C m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.55
_cell_length_b                   8.55
_cell_length_c                   4.13
_cell_volume                     301.913
_exptl_crystal_density_diffrn    3.303
_cod_original_formula_sum        'Cd N2 Br2'
_cod_database_code               9008058
_database_code_amcsd 0010562
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide Locality: synthetic
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008059
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
 Locality: synthetic
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_formula_structural     Cd(NH3)2Br2
_chemical_formula_sum            'Br2 Cd N2'
_space_group_IT_number           21
_symmetry_space_group_name_Hall  'C 2 2'
_symmetry_space_group_name_H-M   'C 2 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.55
_cell_length_b                   8.55
_cell_length_c                   4.13
_cell_volume                     301.913
_exptl_crystal_density_diffrn    3.303
_cod_original_formula_sum        'Cd N2 Br2'
_cod_database_code               9008059
_database_code_amcsd 0010563
Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
MacGillavry, C. H.; Bijvoet, J. M.; Zeitschrift fur Kristallographie 94 (1936) 231–245; doi:

data_9008060
_publ_section_title
;
 Die kristallstruktur der cadmium-und quecksilber-diammin-dihalogenide
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              231
_journal_page_last               245
_journal_volume                  94
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_structural     Hg(NH3)2Cl2
_chemical_formula_sum            'Cl2 Hg N2'
_space_group_IT_number           65
_symmetry_space_group_name_Hall  '-C 2 2'
_symmetry_space_group_name_H-M   'C m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.12
_cell_length_b                   8.12
_cell_length_c                   4.06
_cell_volume                     267.694
_database_code_amcsd             0010564
_exptl_crystal_density_diffrn    3.716
_cod_original_formula_sum        'Hg N2 Cl2'
_cod_database_code               9008060
_amcsd_formula_title             Hg(NH3)2Cl2
The structure of braggite and palladium sulphide Locality: synthetic
Gaskell, T. F.; Zeitschrift fur Kristallographie 96 (1937) 203–213; doi:

data_9008061
_publ_section_title
;
 The structure of braggite and palladium sulphide
 Locality: synthetic
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              203
_journal_page_last               213
_journal_volume                  96
_journal_year                    1937
_chemical_formula_sum            'Pd S'
_chemical_name_mineral           Vysotskite
_space_group_IT_number           84
_symmetry_space_group_name_Hall  '-P 4c'
_symmetry_space_group_name_H-M   'P 42/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.43
_cell_length_b                   6.43
_cell_length_c                   6.63
_cell_formula_units_Z            8
_cell_volume                     274.117
_exptl_crystal_density_diffrn    6.711
_cod_database_code               9008061
_cod_duplicate_entry 1011155
The Crystal Structure of Valentinite (Orthorhombic Sb~2~O~3~)
Buerger, M. J.; Hendricks, S. B.; Zeitschrift f"ur Kristallographie - Crystalline Materials 98 (1938) 1–30; doi:10.1524/zkri.1938.98.1.1

data_9008062
_publ_section_title
;
 The Crystal Structure of Valentinite (Orthorhombic Sb~2~O~3~)
;
_journal_issue                   1-6
_journal_name_full
;
 Zeitschrift f"ur Kristallographie - Crystalline Materials
;
_journal_page_first              1
_journal_page_last               30
_journal_paper_doi               10.1524/zkri.1938.98.1.1
_journal_volume                  98
_journal_year                    1938
_chemical_formula_sum            'O3 Sb2'
_chemical_name_mineral           Valentinite
_space_group_IT_number           56
_symmetry_space_group_name_Hall  '-P 2ab 2ac'
_symmetry_space_group_name_H-M   'P c c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.92
_cell_length_b                   12.46
_cell_length_c                   5.42
_cell_formula_units_Z            4
_cell_volume                     332.263
_database_code_amcsd             0010568
_exptl_crystal_density_diffrn    5.827
_cod_original_formula_sum        'Sb2 O3'
_cod_database_code               9008062
Uber die struktur des durangit NaAlF[AsO~4~] Locality: Durango, Mexico
Kokkoros, P.; Zeitschrift für Kristallographie - Crystalline Materials 99 (1938) 38–49; doi:10.1524/zkri.1938.99.1.38

data_9008063
_publ_section_title
;
 Uber die struktur des durangit NaAlF[AsO~4~]
 Locality: Durango, Mexico
;
_journal_issue                   1-6
_journal_name_full
;
 Zeitschrift f\"ur Kristallographie - Crystalline Materials
;
_journal_page_first              38
_journal_page_last               49
_journal_paper_doi               10.1524/zkri.1938.99.1.38
_journal_volume                  99
_journal_year                    1938
_chemical_formula_sum            'Al As F Na O4'
_chemical_name_mineral           Durangite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.22
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.53
_cell_length_b                   8.46
_cell_length_c                   7.00
_cell_volume                     349.845
_exptl_crystal_density_diffrn    3.947
_cod_original_formula_sum        'Na Al As O4 F'
_cod_database_code               9008063
_cod_duplicate_entry 1011040
Gitterumwandlungen im system Cu2-x Se
Borchert, W.; Zeitschrift fur Kristallographie 106 (1945) 5–24; doi:10.1524/zkri.1945.106.1.5

data_9008064
_publ_section_title
;
 Gitterumwandlungen im system Cu2-x Se
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              5
_journal_page_last               24
_journal_paper_doi               10.1524/zkri.1945.106.1.5
_journal_volume                  106
_journal_year                    1945
_chemical_formula_sum            'Cu2 Se'
_chemical_name_mineral           Berzelianite
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.840
_cell_length_b                   5.840
_cell_length_c                   5.840
_cell_formula_units_Z            4
_cell_volume                     199.177
_database_code_amcsd             0010573
_exptl_crystal_density_diffrn    6.871
_cod_database_code               9008064
Gitterumwandlungen im System Cu2-x Se
Borchert, W.; Zeitschrift fur Kristallographie 106 (1945) 5–24; doi:10.1524/zkri.1945.106.1.5

data_9008065
_publ_section_title
;
 Gitterumwandlungen im System Cu2-x Se
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              5
_journal_page_last               24
_journal_volume                  106
_journal_year                    1945
_chemical_formula_sum            'Cu1.8 Se'
_chemical_name_mineral           Berzelianite
_chemical_compound_source        'sample or refienement with low Cu1 occupancy'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.729
_cell_length_b                   5.729
_cell_length_c                   5.729
_cell_formula_units_Z            4
_cell_volume                     188.034
_exptl_crystal_density_diffrn    6.830
_cod_database_code               9008065
_journal_paper_doi 10.1524/zkri.1945.106.1.5
_database_code_amcsd             0010574
Gitterumwandlungen im System Cu~2-x~Se
Borchert, W.; Zeitschrift fur Kristallographie 106 (1945) 5–24; doi:10.1524/zkri.1945.106.1.5

data_9008066
_publ_section_title
;
 Gitterumwandlungen im System Cu~2-x~Se
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              5
_journal_page_last               24
_journal_paper_doi               10.1524/zkri.1945.106.1.5
_journal_volume                  106
_journal_year                    1945
_chemical_formula_sum            'Cu1.8 Se'
_chemical_name_mineral           Berzelianite
_chemical_compound_source        'sample or refienement with high Cu1 occupancy'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.729
_cell_length_b                   5.729
_cell_length_c                   5.729
_cell_formula_units_Z            4
_cell_volume                     188.034
_cod_database_code               9008066
_database_code_amcsd             0010575
Gitterumwandlungen im System Cu~2-x~Se
Borchert, W.; Zeitschrift fur Kristallographie 106 (1945) 5–24; doi:10.1524/zkri.1945.106.16.5

data_9008067
_publ_section_title
;
 Gitterumwandlungen im System Cu~2-x~Se
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              5
_journal_page_last               24
_journal_paper_doi               10.1524/zkri.1945.106.16.5
_journal_volume                  106
_journal_year                    1945
_chemical_formula_sum            'Cu1.8 Se'
_chemical_name_mineral           Berzelianite
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.729
_cell_length_b                   5.729
_cell_length_c                   5.729
_cell_formula_units_Z            4
_cell_volume                     188.034
_database_code_amcsd             0010576
_exptl_crystal_density_diffrn    6.830
_cod_database_code               9008067
Die kristallstruktur des bixbyits (Fe,Mn)2O3
Dachs, H.; Zeitschrift fur Kristallographie 107 (1956) 370–395; doi:

data_9008068
_publ_section_title
;
 Die kristallstruktur des bixbyits (Fe,Mn)2O3
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              370
_journal_page_last               395
_journal_volume                  107
_journal_year                    1956
_chemical_formula_sum            'Fe Mn O3'
_chemical_name_mineral           Bixbyite
_space_group_IT_number           206
_symmetry_space_group_name_Hall  '-I 2b 2c 3'
_symmetry_space_group_name_H-M   'I a -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   9.40
_cell_length_b                   9.40
_cell_length_c                   9.40
_cell_formula_units_Z            16
_cell_volume                     830.584
_database_code_amcsd             0010577
_exptl_crystal_density_diffrn    5.079
_cod_original_sg_symbol_H-M      'I a 3'
_cod_original_formula_sum        '(Fe Mn) O3'
_cod_database_code               9008068
The crystallography of eucairite, CuAgSe Sample: orthorhombic subcell
Frueh, A. J.; Czamanske, G. K.; Knight, C.; Zeitschrift fur Kristallographie 108 (1957) 389–396; doi:10.1524/zkri.1957.108.5-6.389

data_9008069
_publ_section_title
;
 The crystallography of eucairite, CuAgSe
 Sample: orthorhombic subcell
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              389
_journal_page_last               396
_journal_paper_doi               10.1524/zkri.1957.108.5-6.389
_journal_volume                  108
_journal_year                    1957
_chemical_compound_source        'Skrikerum, Sweden'
_chemical_formula_sum            'Ag Cu Se'
_chemical_name_mineral           Eucairite
_space_group_IT_number           59
_symmetry_space_group_name_Hall  '-P 2ab 2a'
_symmetry_space_group_name_H-M   'P m m n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.105
_cell_length_b                   4.07
_cell_length_c                   6.31
_cell_formula_units_Z            2
_cell_volume                     105.423
_database_code_amcsd             0010578
_exptl_crystal_density_diffrn    7.887
_cod_original_sg_symbol_H-M      'P m m n'
_cod_original_formula_sum        'Cu Ag Se'
_cod_database_code               9008069
The crystallography of eucairite, CuAgSe Sample: tetragonal subcell
Frueh, A. J.; Czamanske, G. K.; Knight, C.; Zeitschrift fur Kristallographie 108 (1957) 389–396; doi:10.1524/zkri.1957.108.5-6.389

data_9008070
_publ_section_title
;
 The crystallography of eucairite, CuAgSe
 Sample: tetragonal subcell
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              389
_journal_page_last               396
_journal_paper_doi               10.1524/zkri.1957.108.5-6.389
_journal_volume                  108
_journal_year                    1957
_chemical_compound_source        'Skrikerum, Sweden'
_chemical_formula_sum            'Ag Cu Se'
_chemical_name_mineral           Eucairite
_space_group_IT_number           129
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.083
_cell_length_b                   4.083
_cell_length_c                   6.31
_cell_formula_units_Z            2
_cell_volume                     105.193
_database_code_amcsd             0010579
_exptl_crystal_density_diffrn    7.905
_cod_original_sg_symbol_H-M      'P 4/n m m'
_cod_original_formula_sum        'Cu Ag Se'
_cod_database_code               9008070
The crystal structure of livingstonite, HgSb4S8
Niizeki, N.; Buerger, M. J.; Zeitschrift fur Kristallographie 109 (1957) 129–157; doi:

data_9008071
_publ_section_title
;
 The crystal structure of livingstonite, HgSb4S8
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              129
_journal_page_last               157
_journal_volume                  109
_journal_year                    1957
_chemical_compound_source        'Guerrido, Mexico'
_chemical_formula_sum            'Hg S8 Sb4'
_chemical_name_mineral           Livingstonite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-A 2ya'
_symmetry_space_group_name_H-M   'A 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.20
_cell_angle_gamma                90
_cell_length_a                   30.25
_cell_length_b                   4
_cell_length_c                   21.48
_cell_formula_units_Z            8
_cell_volume                     2519.666
_database_code_amcsd             0010580
_exptl_crystal_density_diffrn    4.978
_cod_original_formula_sum        'Hg Sb4 S8'
_cod_database_code               9008071